- Email: [email protected]

Journal of Magnetism and Magnetic Materials 272–276 (2004) e1459–e1463

Spin-dependent transport in magnetic nanostructures S. Maekawa* Institute for Materials Research, Tohoku University, Sendai 980-8577, Japan

Abstract Recent progress in physics on spin-dependent transport in magnetic nanostructures is reviewed. Special attention is paid to the spin accumulation and spin current caused by spin injection into non-magnetic metals and semiconductors and superconductors. A variety of phenomena induced in nano-superconductor/ferromagnet devices are proposed, examining the spin–charge separation in superconductors. r 2004 Elsevier B.V. All rights reserved. PACS: 72.25Ba; 72.25.Hg; 72.25.Mk; 73.40.Gk Keywords: Spin-polarized transport; Spin injection; Spin accumulation; Spin current; Tunneling

1. Introduction Discovery of the so-called giant magnetoresistance (GMR) effect in magnetic multilayers [1,2] in 1988 raised the curtain for an intensive new research effort on magnetic materials and magnetic thin ﬁlms which proﬁted enormously from the application of microfabrication techniques [3]. Semiconductor devices have been the main actors on the electronics stage during the latter half of 20th century. The size of such devices has been getting steadily smaller following the impressive progress in microfabrication techniques. In addition, the physics of such small semiconductor devices, i.e., mesoscopic physics, has emerged as a subject of study in its own right. It is also relevant to remember the considerable quantity of new physics which has emerged since the discovery of high-temperature superconductors in 1986. In the latter ﬁeld, one of the main concerns is the behavior of spin and charge and their interactions. On the other hand, to date in semiconductor devices only the movement of charge has found application with spin being usually considered as an irrelevant degree of freedom. The discovery of GMR signalled a starting *Tel.: +81-22-215-2005; fax: +81-22-215-2066. E-mail address: [email protected] (S. Maekawa).

point for the physics and application of the interaction between spin and charge and shed light to the spinpolarized tunneling [4,5] which was studied in advance to GMR. Here, I would like to review the new physics of spin-dependent transport in magnetic nanostructures. Special attention is paid to the spin accumulation and spin current caused by spin injection into non-magnetic metals and semiconductors and superconductors. Examining the spin–charge separation in superconductors [6], a variety of phenomena induced in nanosuperconductor/ferromanget devices are proposed.

2. Spin accumulation Let us consider a double tunnel junction device shown in Fig. 1(a), where two ferromagnetic electrodes and a non-magnetic island are separated by two tunnel barriers. In the device, the magnetic moments of two ferromagnetic electrodes are taken to be antiparallel and the electric current is introduced from the left electrode. In Fig. 1(b), the schematic electronic structure is presented. Here, electrons with up spin mainly come into the central island from the left electrode, whereas electrons with down spin mainly go out from the island to the right. As a result, the spin imbalance occurs in the

0304-8853/$ - see front matter r 2004 Elsevier B.V. All rights reserved. doi:10.1016/j.jmmm.2004.04.091

ARTICLE IN PRESS S. Maekawa / Journal of Magnetism and Magnetic Materials 272–276 (2004) e1459–e1463

∆ /∆ 0

(a)

∆P

1.0

1.0

∆ AP

δµs /∆ 0

e1460

δµs

AP

0.5

0.5 0

0 (b)

G/GPN

1.5

GAP

GP

1.0 0.5

Vc

0

TMR (%)

(c)

Fig. 1. (a) Double tunnel junction comprising two ferromagnets (FM) and a superconductor (SC) separated by insulating barriers. R1 and R2 are the tunnel resistances of the left and right junctions with the voltage drops, V1 and V2 ; across the barriers (V ¼ V1 þ V2 is the total voltage drop across the entire double tunnel junction). Schematic diagram of the densities of states of FMs (left and light) and SC (middle) in the antiparallel alignment of magnetizations of FMs are shown when SC is in the normal state (b) and in the superconducting state (c) dms denotes the shift in the chemical potentials of the spin subbands.

island with a size smaller than the spin diffusion length ðls Þ; when electrons pass through it within the time less than the spin-relaxation time ðts Þ: Since the magnetization is given by the difference between the numbers of electrons with up and down spins times the Bohr magneton ðmB Þ; the island is magnetized by the electric current. This is called spin accumulation. Spin accumulation causes the tunnel magnetoresistance (TMR) [7–12]. In a double tunnel junction device with two equivalent ferromagnetic electrodes, the spin polarization being P; and two equal tunnel barriers, the TMR is given by TMR ¼ P2 =ð1 P2 Þ;

ð1Þ

which is half of that in the usual ferromagnetic tunnel junctions, i.e., TMR ¼ 2P2 =ð1 P2 Þ [4,5,13–16]. Therefore, the spin accumulation may be examined by using TMR. Recently, the TMR due to the spin accumulation has been studied in GaMnAs/GaAs/GaMnAs double tunnel junction devices [12]. When the central island in Fig. 1(a) becomes superconducting, the competition between spin accumulation and superconductivity occurs as depicted in Fig. 1(c). In the superconducting

40 20 0 –20 –40

0

1

2

3

eV/2∆ 0 Fig. 2. (a) Superconducting gaps, DP and DAP ; for the parallel (P) and antiparallel (AP) alignments of magnetizations, respectively, and the half of the spin splitting between the spin-up and spin-down bands in the AP alignment, dmAP s : (b) Tunnel conductances, GP and GAP ; for the P and AP alignments, respectively. (c) Tunnel magnetoresistance (TMR). Thin dashed line indicates TMR ¼ P2 =ð1 P2 Þ in the normal state. The values P ¼ 0:4 and T=Tc ¼ 0:5 are taken for all curves.

state, there appears the superconducting gap ðDÞ; which competes with the spin accumulation. In Fig. 2(a), the theoretical results of the shift of the Fermi level ðdms Þ due to spin accumulation and D are presented as functions of bias voltage ðV Þ in the double tunnel junction device where the magnetic moments in the electrodes are antiparallel. When the bias voltage becomes of the order of the gap, eV =2BD=P; the superconductivity is suppressed [10]. In Fig. 2(b), the tunnel conductances, GAP and GP ; are shown in the device with antiparallel and parallel magnetic moments, respectively. For the antiparallel magnetic moments, the superconductivity is suppressed at V ¼ Vc and the conductance jumps. The TMR in the device is given in Fig. 2(c), where the dashed line shows the value given by Eq. (1). We note that the TMR oscillates as a function of V since D depends on spin accumulation [17–19]. The suppression of the superconducting gap by spin accumulation may be observed by the superconducting critical current, Jc ;

ARTICLE IN PRESS S. Maekawa / Journal of Magnetism and Magnetic Materials 272–276 (2004) e1459–e1463

(a)

Jc /Jc0

1

P1= 0.8 P2= 0.8

0

– 0.5

0

(b)

0.5

P1= 0.8 P2= 0.4

Jc /Jc0

1

0

–1

0

(c) 1

T/Tc = 0.9

1

e1461

respectively, in Fig. 3(c), where Nd1x Srx MnO3 is a ferromagnetic electrode and YBa2 Cu3 O7 is a hightemperature superconductor with Tc ¼ 89 K: As noted above, the shift of the Fermi level ðdms Þ due to spin accumulation competes with the superconductivity, which disappears at Vc B2D=eP: It is also known that the superconductivity is suppressed by an applied magnetic ﬁeld (Pauli paramagnetic effect). In this case, the critical ﬁeld is given by Hc B2D=mB : By comparing these two effects, we ﬁnd that the bias voltage of 0:1 V corresponds to the magnetic ﬁelds of the order of 102 T for superconductivity. It is very hard to suppress the high-temperature superconductivity by an applied magnetic ﬁeld, since it is too large to access it in the usual experimental conditions. On the other hand, the bias voltage of the order of 0:1 V may be obtained easily. This fact suggests potentials for application of spin accumulation in various ﬁelds.

P1= 0.8 P2= 0

Jc /Jc0

3. Spin injection devices 0.95 0.99 0

– 0.5

0

0.5

Iinj /(∆0 /eRT) Fig. 3. Critical current Jc as a function of injection current Iinj for the spin polarizations P1 of FM1 and different values of P2 of FM2 at T=Tc ¼ 0:9: (a) P1 ¼ 0:8 and P2 ¼ 0:8; (b) P1 ¼ 0:8 and P2 ¼ 0:4; and (c) P1 ¼ 0:8 and P2 ¼ 0: Open circles indicate the critical current at T ¼ 80; 84 and 87 K ðTc B89 KÞ in Au=YBa2 Cu3 O7 =LaAlO3 =Nd2=3 Sr1=3 MnO3 junctions [21].

following the relation, Jc pD3 [10,20–24]. In Fig. 3, Jc normalized by that at zero temperature, Jc0 ; is plotted as a function of the injected current, Iinj ; at T=Tc ¼ 0:9; the temperature ðTÞ being normalized by the critical temperature ðTc Þ: Here, the spin polarization of one of the ferromagnetic electrodes is taken to be P1 ¼ 0:8 and that of the other one is chosen to be the values, P2 ¼ 0; 0.4 and 0.8. The tunnel resistance of both tunnel barriers are equal and is taken to be RT : For the tunnel device with the same ferromagnetic electrodes ðP1 ¼ P2 Þ; the superconductivity is strongly suppressed for the antiparallel magnetic moments, whereas it is not for the parallel moments as seen in Fig. 3(a). On the other hand, for the device with different ferromagnets ðP1 aP2 Þ; the superconductivity is suppressed even for the parallel moments since spins coming into and going out of the island is not equal (Fig. 3(b)). When one of the electrodes is non-magnetic, P2 is equal to zero (Fig. 3(c)). The experimental result obtained in Nd1x Srx MnO3 =YBa2 Cu3 O7 =Au devices [21] and theoretical ones are shown by circles and solid lines,

Johnson and Silsbee in 1985 [25] and Johnson in 1993 [26] have proposed a three-terminal device shown in Fig. 4(a), which consists of a non-magnetic metal (P) and two ferromagnets (F1 and F2). Let us consider that both F1 and F2 are half-metallic, for simplicity. Then, electrons with up spin are injected from F1 into P as seen in Fig. 4(b). As a result, the Fermi level with up spin in P is different from that with down spin. Therefore, the voltage ðV2 Þ depends on whether the magnetic moment of F2 is parallel or antiparallel to that of F1 [27–30]. Recently, well-deﬁned three-terminal devices were prepared by using the microfabrication technique [31,32]. Here, it is important that the size of the devices is

F1 P F2

(a)

VF2 I (b)

F1 E

P Ispin

F2, parallel E

E

µF1

µFP

Vs N (E)

2δµ s

F2, antiparallel µF2

2RsI

N (E)

Fig. 4. (a) Three-terminal device introduced by Johnson [26]. Arrows in F1 and F2 refer to the magnetization orientation. (b) Diagram of the densities of states of the ferromagnet (F1)/paramagnet (P)/ferromagnet (F2) system in (a).

ARTICLE IN PRESS S. Maekawa / Journal of Magnetism and Magnetic Materials 272–276 (2004) e1459–e1463

e1462

smaller than the spin diffusion length ðls Þ; which is less than 1 mm in the usual non-magnetic metals. Since the signal in such spin injection devices is obtained as the voltage induced by the electric current, a low-carrier material in the non-magnetic part will provide an opportunity for obtaining the larger signal. Therefore, semiconductors such as GaAs with long spin diffusion length may be good candidates in the devices [33–36]. We note that superconductors are low-carrier systems for spin, since spin is carried by quasi-particles whereas charge is by Cooper pairs. Thus, the large spin injection signal is also expected in the devices with superconductors [33].

4. Anomalous Hall effect Anomalous Hall effect in a ferromagnet is caused by spin-polarized current scattered by the spin–orbit interaction at impurities [37–40]. In other words, spin current shifts to charge current perpendicular to the applied bias voltage by the scattering [37]. Let us consider a double tunnel junction device in Fig. 5, where two electrodes are made of the same ferromagnet with magnetic moments perpendicular to the ﬁlm plane (z-direction). The current ðIinj Þ is injected from the left electrode to the nonmagnetic central one (x-direction). In this case, the charge and spin currents, respectively, are expressed as Icharge ¼ Im þ Ik ;

ð2Þ

Ispin ¼ Im Ik ¼ PIinj ;

ð3Þ

where Im and Ik are the current with spin up and down, respectively, and P is the spin polarization in the ferromagnetic electrodes. The Hall current is induced perpendicular to the injected current (y-direction) and the Hall voltage is given by VH p~ z~ I spin ¼ ~ z P~ I inj :

ð4Þ +

VH +++++

FM

FM

j↑

y x

I inj

+++++

SC

j↓

I inj m//z

m//z

-----

-----

VH− Fig. 5. Spin injection device of a double tunnel junction FM/ SC/FM in the parallel magnetic moments of FMs, in which a nonequilibrium Hall voltage VH is induced in the transverse direction by injection of spin-polarized current.

It is interesting to see the Hall voltage in the superconducting state. As mentioned in the previous section, the charge current is carried by Cooper pairs and is not affected by impurities. Since impurity scattering occurs only for quasi-particles which carry spin current, the Hall effect in superconductors proves that the anomalous Hall effect is due to spin current but not charge [40].

5. Conclusion Recent progress in microfabrication techniques has brought spin-electronics devices of the order of or smaller than the spin diffusion length ðls Þ [41], which provide a variety of spin-dependent phenomena due to spin accumulation and spin current. The phenomena also depend on the geometry of the devices. Spindependent transport in magnetic nanostructures is based on the physics of the interaction between spin and charge. In this sense, the spin–charge separation of electrons is a starting point for the physics of spinelectronics.

Acknowledgements I would like to thank S. Takahashi, H. Imamura, T. Yamashita and J. Martinek for their continuous collaboration in this ﬁeld. This work has been supported by a Grant-in-Aid for Scientiﬁc Research from MEXT and CREST.

References [1] M.N. Baibich, et al., Phys. Rev. Lett. 61 (1988) 2472. [2] G. Binash, et al., Phys. Rev. B 39 (1989) 4828. [3] S. Maekawa, T. Shinjo (Eds.), Spin Dependent Transport in Magnetic Nanostructures, Taylor & Francis, London, New York, 2002. [4] M. Julliere, Phys. Lett. 54 A (1975) 225. [5] S. Maekawa, U. Gafvert, IEEE Trans. Magn. 18 (1982) 707. [6] J.R. Schrieffer M. Tinkham, Rev. Mod. Phys. 71 (1999) 313. [7] J. Barnas, A. Fert, EuroPhys. Lett. 44 (1998) 85. [8] A. Brataas, Y.V. Nazarov, J. Inoue, G.E.W. Bauer, Phys. Rev. B 59 (1999) 93. [9] H. Imamura, S. Takahashi, S. Maekawa, Phys. Rev. B 59 (1999) 6017. [10] S. Takahashi, H. Imamura, S. Maekawa, Phys. Rev. Lett. 82 (1999) 3911; S. Takahashi, H. Imamura, S. Maekawa, J. Appl. Phys. 87 (2000) 5227. [11] J. Martinek, J. Barnas, A. Fert, S. Maekawa, G. Schon, J. Appl. Phys. 93 (2003) 8265. [12] R. Mattana, et al., Phys. Rev. Lett. 90 (2003) 166601.

ARTICLE IN PRESS S. Maekawa / Journal of Magnetism and Magnetic Materials 272–276 (2004) e1459–e1463 [13] J.S. Moodera, et al., Phys. Rev. Lett. 74 (1995) 3273. [14] T. Miyazaki, N. Tezuka, J. Magn. Magn. Mater. 139 (1995) L231. [15] J.C. Slonczewski, Phys. Rev. B 39 (1989) 6995. [16] S S. P. Parkin, et al., J. Appl. Phys. 85 (1999) 5828. [17] T. Miyazaki, Private Communication. [18] J. Johansson, et al., J. Appl. Phys. 93 (2003) 8650. [19] T. Ono, Private Communication. [20] V.A. Vas’ko, et al., Phys. Rev. Lett. 78 (1997) 1134. [21] Z.W. Dong, et al., Appl. Phys. Lett. 71 (1997) 1718. [22] N.-C. Yeh, et al., Phys. Rev. B 60 (1999) 10522. [23] J.Z. Liu, et al., Physica C 357–360 (2001) 1614. [24] C.D. Chen, et al., Phys. Rev. Lett. 88 (2002) 047004. [25] M. Johnson, R.H. Silsbee, Phys. Rev. Lett. 55 (1985) 1790; M. Johnson, R.H. Silsbee, Phys. Rev. Lett. 60 (1988) 377. [26] M. Johnson, Phys. Rev. Lett. 70 (1993) 2142. [27] T. Valet, A. Fert, Phys. Rev. B 48 (1993) 7099. [28] A. Fert, S.F. Lee, Phys. Rev. B 53 (1996) 6554.

e1463

[29] S. Hershﬁeld, H.L. Zhao, Phys. Rev. B 56 (1997) 3296. [30] M. Johnson, J. Byers, Phys. Rev. B 67 (2003) 125112. [31] F.J. Jedema, et al., Nature (London) 410 (2001) 345; F.J. Jedema, et al., Nature (London) 416 (2002) 713; F.J. Jedema, et al., Phys. Rev. B 67 (2003) 085319. [32] J.-M. George, A. Fert, G. Faini, Phys. Rev. B 67 (2003) 012410. [33] S. Takahashi, S. Maekawa, Phys. Rev. B 67 (2003) 052409. [34] A. Fert, H. Jaffre`s, Phys. Rev. B 64 (2001) 184420. [35] E.I. Rashba, Phys. Rev. B 62 (2000) R16267. [36] G. Schmidt, et al., Phys. Rev. B 62 (2000) R4790. [37] J.E. Hirsch, Phys. Rev. Lett. 83 (1999) 1834. [38] S. Zhang, Phys. Rev. Lett. 85 (2000) 393. [39] Y. Otani, et al., J. Magn. Magn. Mater. 239 (2002) 135. [40] S. Takahashi, S. Maekawa, Phys. Rev. Lett. 88 (2002) 116601. [41] T. Yamashita, H. Imamura, S. Takahashi, S. Maekawa, Phys. Rev. B 65 (2002) 172509.

Copyright © 2021 COEK.INFO. All rights reserved.